| ||Format||Pages||Price|| |
|8||$50.00||  ADD TO CART|
|Hardcopy (shipping and handling)||8||$50.00||  ADD TO CART|
|Standard + Redline PDF Bundle||16||$60.00||  ADD TO CART|
Significance and Use
4.1 Transparent plastic materials, when used as windows or enclosures, are subject to wiping and cleaning; hence the maintenance of optical quality of a material after abrasion is important. It is the purpose of this test method to provide a means of estimating the resistance of such materials to this type and degree of abrasion.
4.2 Although this test method does not provide fundamental data, it is suitable for grading materials relative to this type of abrasion in a manner which correlates with service.
4.3 Comparison of interlaboratory data or the specification of a “haze” value has no significance if the hazemeter requirements given in are not used. This is because light diffused from the surface of a Taber track is scattered at a narrow angle ( and ) while light diffused internally by a specimen is scattered at a wide angle. In many hazemeters, when a diaphragm is inserted to limit the light beam to the width of the abraded track, the specular beam at the exit port becomes smaller. The dark annulus will then be greater than the 0.023 rad ± 0.002 rad (1.3° ± 0.1°) requirements of Test Method . Since a large percentage of the narrow-angle forward-scattered light will not impinge on the sphere wall, “haze” readings become smaller. For hazemeters that have not been properly adjusted, the magnitude of this reduction is dependent both on the integrating sphere diameter and the reduction of the entrance beam.
FIG. 1 Light Scattering from Surface of Abraded Tracks (Photograph)
Note 1: This photograph shows light pattern of the scattering from the surface of a Taber abraded specimen. The circles show how increasing the 1.3° dark annulus dramatically changes the amount of light impacting the sphere wall.
FIG. 2 Light Scattering from Surface of Abraded Tracks (Graph)
Note 1: This graph shows goniophotometric curves for Taber abraded tracks. The specular angle of transmission is at 180°.
4.4 For many materials, there may be a specification that requires the use of this test method, but with some procedural modifications that take precedence when adhering to the specification. Therefore, it is advisable to refer to that material specification before using this test method. Table 1 of Classification System lists the ASTM materials standards that currently exist.
4.5 For some materials, abrasion tests utilizing the Taber abraser may be subject to variation due to changes in the abrasive characteristics of the wheel during testing.
4.5.1 Depending on abradant type and test specimen, the wheel surface may change (that is, become clogged) due to the transfer of coating or other materials from test specimens and must be cleaned at frequent intervals.
4.5.2 The type of material being tested and the number of test cycles being run is known to sometimes influence the temperature of the running surface of the wheel with an effect on the final haze measurement. To reduce any variability due to this temperature effect, stabilize the wheels surface temperature prior to performing actual measurements. This shall be accomplished by conducting multiple refacings on an ST-11 refacing stone, followed by a test on the sample material to be tested (with results to be discarded).
1.1 This test method describes a procedure for estimating the resistance of transparent plastics to one kind of surface abrasion by measuring the change in optical properties.
1.2 Abrasive damage is numerically quantified by calculating the difference in haze percentage in accordance with Test Method between an abraded and unabraded specimen.
1.3 The values stated in SI units are to be regarded as standard. The values given in parentheses are for information only.
Note 1: This test method is equivalent in the measurement of resistance to abrasion of ISO 3537, Section 8 and ISO 15082, Section 11, but is not equivalent in any other measurement or section. This test method is not equivalent to ISO 9352, and results cannot be directly compared between the two methods.
Note 2: This test method is similar to SAE J3097Z26, Test 12.
Note 3: Prior attempts to employ the Taber Abraser for volume loss determinations of various plastics have been unsuccessful because of excessively large coefficients of variation attributed to the data. Insufficient agreement among the participating laboratories has rendered the use of volume loss procedure inadvisable as an ASTM test method.
Note 4: For determining the resistance to abrasion of organic coatings by weight loss, reference is made to Test Method , which uses more aggressive CS-10 or CS-17 abrasive wheels.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.5 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D883 Terminology Relating to Plastics
D1003 Test Method for Haze and Luminous Transmittance of Transparent Plastics
D4000 Classification System for Specifying Plastic Materials
D4060 Test Method for Abrasion Resistance of Organic Coatings by the Taber Abraser
E456 Terminology Relating to Quality and Statistics
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
G195 Guide for Conducting Wear Tests Using a Rotary Platform Abraser
ISO StandardsISO 15082 ISO 3537 ISO 9352
ICS Number Code 83.080.01 (Plastics in general)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D1044-19, Standard Test Method for Resistance of Transparent Plastics to Surface Abrasion by the Taber Abraser, ASTM International, West Conshohocken, PA, 2019, www.astm.orgBack to Top